Ricardo Pinto1 , António L Amaral 1,2 , Eugénio C Ferreira1 , Manuel Mota1, Manuel Vilanova 3,4 , Katia Ruel5 and Miguel Gama
BMC Biotechnology Research article
Quantification of the CBD-FITC conjugates surface coating on cellulose fibres
1 Ricardo Pinto , António L Amaral , Eugénio C Ferreira , Manuel Mota , 3,4
1 Manuel Vilanova , Katia Ruel and Miguel Gama* 1 Address:
IBB-Institute for Biotechnology and Bioengineering, Centre of Biological Engineering, Universidade do Minho, Campus de Gualtar,2 3 4710-057 Braga, Portugal, Departamento de Tecnologia Química, ESTIG, IPB, Apartado 1038, 5301-854 Bragança, Portugal, 4 ICBAS – Instituto de Ciências Biomédicas de Abel Salazar, Largo do Professor Abel Salazar 2, 4099-003 Porto, Portugal, 5 IBMC – Instituto de Biologia Molecular e Celular, Rua do Campo Alegre, 823, 4150-180 Porto, Portugal and Centre de Recherches sur les Macromolécules Végétales (CERMAV)-UPR CNRS 5301, BP 53, 38041 Grenoble cedex 9, France Email: Ricardo Pinto - email@example.com; António L Amaral - firstname.lastname@example.org; Eugénio C Ferreira - email@example.com; Manuel Mota - firstname.lastname@example.org; Manuel Vilanova - email@example.com; Katia Ruel - Katia.Ruel@cermav.cnrs.fr; Miguel Gama* - firstname.lastname@example.org
- Corresponding author Published: 9 January 2008 Received: 23 January 2007 Accepted: 9 January 2008
BMC Biotechnology 2008, 8:1 doi:10.1186/1472-6750-8-1 © 2008 Pinto et al; licensee BioMed Central Ltd.
This is an Open Access article distributed under the terms of the Creative Commons Attribution Licens which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Abstract Background: Cellulose Binding Domains (CBD) were conjugated with fluorescein isothiocyanate
(FITC). The surface concentration of the Binding Domains adsorbed on cellulose fibres was determined by fluorescence image analysis.
Results: For a CBD-FITC concentration of 60 mg/L, a coating fraction of 78% and 110% was
estimated for Portucel and Whatman fibres, respectively. For a saturating CBD concentration, using -13 2 Whatman CF11 fibres, a surface concentration of 25.2 × 10 mol/mm was estimated, the equivalent to 4 protein monolayers. This result does not imply the existence of several adsorbed protein layers.
Conclusion: It was verified that CBDs were able to penetrate the fibres, according to confocal
microscopy and TEM-immunolabelling analysis. The surface concentration of adsorbed CBDs was greater on amorphous fibres (phosphoric acid swollen) than on more crystalline ones (Whatman CF11 and Sigmacell 20).
Background Cellulose-Binding Domains (CBD) are modules present
Due to its high sensitivity and specificity, fluorescence in most celulases, being responsible for their high affinity analysis has been extensively used in microarray technol- to cellulose crystalline surfaces The CBD used in this ogy [tein diffusion work, produced by limited proteolysis, belongs to cellobi- . Three tyrosine residues define a flat based techniques is protein quantification. The use of surface, which may be responsible for the affinity to cellu- either non-coein has a single amine, the N-terminal increased the detection sensitivity to as low as 40 ng/mL. of the linker region, which allows a specific reaction with fluorescein isothiocyanate (FITC). The conjugation with FITC does not affect the CBD interaction with cellulose, since the N-terminal is isolated from the cellulose inter- acting part of the protein. Indeed, the conjugation of FITC does not modify the CBD adsorption isoth
Since there is only one amine group present in the CBD, the stoichiometry of the conjugation reaction is 1:1. The FITC fluorophore has been attached to antibodiesg domains . Several recombinant CBDs, fused to different proteins, have been produced, as recently reviewed by Shoseyov et al.. Cellulose-Binding Domains (CBD) have been used to tar- get functional molecules to cellulose-containing materials that these applica- tions are related to surface effects, in this work we attempted to quantify the CBD surface coverage of cellu- lose fibres, using the approach based on the use of CBD- FITC previously developed. Our aim was to quantify the protein adsorbed on cellulose fibres and, more specifi- cally, the surface concentration of CBD. This value could, alternatively, be estimated by measuring the specific sur- face area, by means of the BET isotherm The presence of CBDs in the interior of the fibres was also investigated.
Results and Discussion
In a previous wo affect the technical properties of paper fibres (secondary fibres from the paper mill Portucel). The concentration of CBDs, used in those experiments, was in the range of 1–2 mg of CBD per gram of fibres. It is arguable whether this rela- tively low amount of protein is sufficient to cause modifi- cations in the fibres' interfacial properties. This would probably imply a substantial coating of the fibres by CBDs. In this work, we analyzed fibres from Portucel treated with CBDs conjugated to FITC, and attempted to estimate the percentage of surface coverage. Fibres treated with only CBDs didn't present any fluorescence. As may be observed in Fi, the fibres do not display a uni- form distribution of fluorescence. This may be due to the chemical heterogeneity (lignin/hemicellulose) and/or to the variable crystas with less intense fluorescence in the picture were selected for CBD- FITC quantification, since these regions are expected to be more crystalline (Pinto et al., unpublished). The detected fluorescence is produced by CBDs adsorbed on both sides of the fibres (top and bottom). Indeed, the fluorescent radiation crosses the fibres with just a slight reduction in intensows a Whatman CF11 fibre, both on bright field and fluorescence microscopy. As it can be observed in the circled area, this cellulose has a rather smooth surface. The extremities of the fibres are expected to have a higher number of fissures and loosen microfibrils, increasing the available area, and conse- quently the adsorbing sites for CB], as indicated by
Portucel and Whatman CF11 fibres treated with CBD-FITC Figure 1
Portucel and Whatman CF11 fibres treated with CBD-FITC. The fibres treated with a concentration of 60 μg/mL (or
2 mg CBD /g fibres ). The images were acquired with an exposure time of 600 ms. The white squares identify the areas selected for analysis. The more fluorescent parts (black regions on the analyzed images) are out of range (calibration shown elsewhere), and were therefore excluded from the analysis. the higher fluorescence emirption of CBDs on Whatman CF11 fibres was analyzed, using a protein concentration of 2 mg/g
. The estimated sur- face concentrations of CBDs adsorbed on Portucel and Whatman CF11 fibr In another experiment, Whatman CF11, amorphous cel- lulose and Sigmacell 20 fibres were allowed to adsorb CBDs from a much more concentrated CBD solution (400 μg/mL), corresponding to 20 mg/gFibres (F concentration is expected to saturate the fibres according to the adsorption isotherm. Considering the size [ of a cellobiohydrolase I CBD (3.0 × 1.8 nm), the density of a CBD monolayer corre- sponds to 3.08 × 10
. It is also considered that the fluorescent signal is produced by CBDs adsorbed on the two sides of the fibres' external surface. Indeed, the accessible area may be much larger than the one corre- sponding to a flat, impenetrable fibre. Therefore, an esti- mate of about 4 layers of CBDs adsorbed in the Whatman CF11 surface results from this reasoning, when the larger concentration of CBDs is used; for a lower CBD concen- tration, a surface coverage of 77% and 110% is estimated, respectively, for Portucel and Whatman fibr dividing the calculated surface concentration by the theo- retical monolayer of CBDs. This is much higher than the expected maximum of one layer of adsorbed CBD, at sat- uration. Although the surface is apparently smooth, the fibres may have irregularities, such as microfissures or holes created bye presence of more or less loose microfibrils, large pores or fissures may substan- tially increase the surface area and the amount of bound proteins, thus leading to a higher fluorescence emission than the theorized monolayer. Indeed, confocal micros- copy reveals that the surface has many irregularities (Fig. other important observation pro- vided by confocal microscopy was that fluorescence in the inner core of the fibres was always superior to the back- ground integ that CBDs may have penetrated into the fibre. As a matter of fact, as shown fluorescent material (CBD- FITC) was detected at all depths of the fibre. This observa- tion is supported by immunolabelling of CBD-treated CF11 fibres . This analysis revealed the presence of CBDs (black spots) in the interior of the fibre. Consider- ing this, we may now explain that the surface concentra- s penetration deep inside the fibres. Another aspect to take into account is that CBDs may not adsorb as a single and well ordered monolayer, but rather as agglom], thereby increasing the average fluorescence per unit area. Never- theless, it is quite probable that the CBD coating of the external surface is rather significant. Amorphous cellulose was prepared, by treating Whatman CF11 with phosphoric acid, which induces the swelling of fibres. As it can be seen in Figure he fibres are larger than the original ones (amorphous Whatman versus Whatman CF11). This swelling effect is due to the disrup- tion or loosening of the microfibrils, thus increasing the volume occupied by the total fibre. As a result, the total surface area available for CBD adsorption increases. Con- sequently, it is expected that the measured CBD fluores- cence would be higher than the one obtained for CF11 fibres, mostly due to an easier penetration of CBD into the fibres structure. This was confirmed, as can be seen in Fig- ge increases about 50% (4 versus 6 layers, respectively for Whatman CF11 and amorphous cellulose). This result can arise either from increased CBD affinity for the more amorphous fibres, or to easier pene- tration, and hence higher concentration in the fibres. Due to the higher fluorescence obtained with these fibres, the
Whatman CF11 images Figure 2 Whatman CF11 images. The characteristic curled struc- ture of the fibres (circle).
Estimated surface concentration of adsorbed CBD Figure 3 Estimated surface concentration of adsorbed CBD.
The estimated fraction of surface coverage is indicated in the figure bars. The values shown are based on the assumption that the protein is adsorbed on the external surface of the fibres only. The values are shown with 95% confidence inter- vals error bars.
Images obtained by fluorescence microscopy of Whatman CF11, amorphous and Sigmacell 20 fibres Figure 4 Images obtained by fluorescence microscopy of Whatman CF11, amorphous and Sigmacell 20 fibres. The
images were obtained before – 1st and 3rd column – and after – 2nd and 4th column – the image analysis of fibres treated with a CBD-FITC concentration of 400 μg/mL. The black areas on the treated images correspond to the fluorescence emission, which is higher than the one used in the calibration. Fluorescence images acquired for 100 ms (CF11) and 80 ms (Amorphous and Sigmacell). majority of the image exceeded the maximum concentra- and confocal microscopy. It seems that a large fraction of tion used in the calibration and it had to be excluded in the adsorbed CBDs actually penetrate the fibres. The sur- the image an face coverage values are, undoubtedly, high enough to jus- tify a change in the fibres' surface properties. CBDs may Sigmacell 20 is obtained by the separation of crushed cel- therefore be used as powerful tools to modulate the fibres' lulose fibres, with an average size of 20 μm. This mechan- surface properties. ical treatment expectedly leads to broken ends or loosen fibrils (amorphous material). Then, the adsorption of Methods
CBD is expected to be higher than with CF11 and compa- rable to the amorphous cellulose (see. Again, the Fluorescein isothiocyanate (FITC), SigmaCell Type 20 and fibres present a high fluorescence emission corresponding Whatman CF11 were obtained from Sigma. Secondary to a high amount of adsorbed CBD: about 5 layers. fibres where kindly supplied by Portucel Viana. All chemi- cals were of the highest purity available in the market.
In this work, the surface concentration of CBD adsorbed Amorphous Cellulose Preparation on cellulose fibres was estimated. The coating values Amorphous cellulose was prepared by treating Whatman obtained were higher than expected, corresponding in CF11 fibres with phosphoric acid. Briefly, 0.17 g of What- theory to several layers (4 to 6) of CBDs adsorbed on the man CF11 were slowly mixed with 10 mL of cold (4°C) external surface. However, it has been demonstrated that phosphoric acid (85%), and left in contact for 5 minutes. the CBDs penetrate the fibres. An important amount of Then, 600 mL of cold water were added and the suspen- CBDs was detected inside the fibres by immunolabelling sion was filtered through a test sieve (mesh width 71 μm,
Figure 5 Images from confocal microscopy
Images from confocal microscopy. Three views of a CF11 fibre are shown, as schematized in the right insertion of figure
c. The insertions d, e and f correspond to the pixels intensity (256 grey levels) obtained at the position indicated by the line
(white circle), at different depths. The adsorption conditions were 20 mg /g , for 30 minutes of contact. Each image cor- CBD Fibre responds to an acquisition thickness of 1 μm. according to DIN 4188). Finally, the fibres were exten- CBD Production sively washed first in tap water and afterwards with dis- The CBDs were prepared according to the following meth-
tilled water. The obtained material was lyophilized and odology: the Celluclast commercial enzymatic prepara- stored. tion (Novozymes A/S, Denmark) was digested with Papain (1:1200, protein basis). The CBDs were separated by ultrafiltration through a 10 kDa membrane (Pellicon 2 TFF System from Millipore, USA) and concentrated by precipitation with ammonium sulphate (Merck, Darm- stadt, Germany). After dialysis, the protein was injected on a Sepharose Fast-Flow gel (Amersham Pharmacia Bio- tech AB, Sweden), and the non-adsorbed protein was col- lected and lyophilized. The purity and identity (CBD from
CBH I) of this protein has been demonstrated by N-terminal sequencing and MALD
The conjugation of CBD with the labelling probe was car- ried out by mixing 20 μg of FITC per mg of CBD (2 mg protein/mL in 0.1 M HEPES buffer, pH 9.0). This solution was incubated overnight in the dark, at room temperature, with magnetic stirring. To eliminate the unbound FITC, the labelled CBD mixture was filtered through a BIO-GEL P-4 (BIO-RAD, Hercules, USA) column, previously equil- ibrated with 50 mM sodium acetate buffer (Panreac, Bar- celona, Spain).
CBD-FITC Adsorption Electron microscopy image of immunolabelling of CBD- treated Whatman CF11 fibres Figure 6
Electron microscopy image of immunolabelling of CBD- Adsorption assays of FITC-labelled CBD were carried out treated Whatman CF11 fibres. at 4°C. The conjugates were allowed to adsorb on cellu- lose fibres (20 g/L, in 50 mM sodium acetate buffer, pH
5.0), with continuous magnetic stirring, in the dark, for 2 hours. The supernatant with unbound CBD was removed by centrifugation at 3219 RCF for 10 minutes (Heraeus Megafuge 1.0R). The fibres were washed with acetate buffer to remove the non-adsorbed CBD-FITC.
Fluorescence microscopy observations were performed in a Zeiss Axioskop microscope (Zeiss, Oberkochen, Ger- many) equipped with a Zeiss AxioCam HRc attached cam- era (Zeiss, Oberkochen, Germany) and using the AxioVision 3.1 software (Zeiss, Oberkochen, Germany). All images were acquired at 1300 × 1030 pixels and 24 bits colour depths (8 bits per channel). The FITC-CBD quanti- fication was performed as described else Confocal observation was performed in an Olympus (Tokyo, Japan) Fluoview 1000 in Laser Scanning mode equipped with a 60× UPLSAPO lens, with a numerical aperture of 1.35 and a pinhole size of 105 μm.
CBD-specific antibodies were produced in a rabbit (Oryc-
) maintained under standard conditions of housing with unrestricted access to food and water; these conditions followed European Union Directive no. 86/609/CEE. Briefly, the rabbit was immunized intrader- mically (i.d.) with a 1:1 suspension of Phosphate Buffered saline (PBS)/Complete Freund's adjuvant containing 500 μg CBD and boosted two weeks later i.d. with a 1:1 sus- pension of PBS/Incomplete Freund's adjuvant containing 500 μg CBD. Blood was collected three weeks after the sec- ond immunization for the preparation of immune serum. Purification of IgG antibodies from this serum sample was performed as follows: the serum sample was equilibrated in a binding buffer (20 mM sodium phosphate, pH 7.0) by overnight dialysis and 3 ml of this preparation was applied to a Protein G HP affinity column (HiTrap, Amer- sham Biosciences, UK). Bound antibodies were eluted with Glycine -HCl buffer, pH 2.7 and recovered in 50 μl of 1 M Tris-HCl pH 9.0 per ml of eluent, according to the manufacturer's instructions. Recovered IgG antibodies were further equilibrated in PBS in a VIVAPORE concen- trator with a 7.5 kDa cutoff membrane (Vivascience, Hanover, Germany) and stored at -80°C in frozen aliq- uots. The anti-CBD antibody titre of this preparation was determined by ELISA. Specific anti-Sap2 or anti CaS anti- bodies in mice sera collected by retrorbital bleeding were quantified by ELISA. Polystyrene microtitre plates (Nunc, Roskilde, Denmark) were coated with 20 μg/ml of CBD and incubated o.n. at 4°C. Wells were then saturated for 1 h at room temperature with 1% BSA in PBS. Serial dilu- tions of the serum samples were then plated and incu- bated for 2 h at room temperature. After washing, bound antibodies were detected by adding alkaline phosphatase- coupled monoclonal goat anti-rabbit-IgG antibody (Southern Biotechnology Associates, Birmingham, ALA, USA) for 30 min at room temperature. Substrate solution containing p-nitrophenyl phosphate (Sigma, St. Louis, USA) was then added after washing and the reaction was stopped by adding 0.1 M EDTA pH 8.0. The absorbance was measured at 405 nm. The ELISA antibody titres were expressed as the reciprocal of the highest dilution giving an absorbance of 0.1 above that of the control (no serum added). The titre of anti CBD antibodies in the purified IgG preparation was of 4014. No antibodies with this spe- cificity were detected in the control sera from non-immu- nized rabbits.
Immunolabelling in Transmission Electron Microscopy
The CBD-treated Whatman CF11 fibres were fixed in a freshly prepared mixture of 0.2% glutaraldehyde (v/v), 2% paraformaldehyde (w/v) in 0.05 M phosphate buffer (pH 7–7.2). Successive periods of vacuum (5 to 10 min) and air inlet were carried out, up to two hours. Afterwards, the fibres were washed 3 × 10 minutes with 0.05 M phos- phate buffer. The samples were then dehydrated through a graded series of ethanol and embedded in London Resin White (hard mixture) polymerized for 24 h at 50°C.
Immunolabelling was done on ultrathin transverse sec- tions (500 Å) floating on plastic rings [ sections were floated on several dilutions of the antiserum in 10 mM Tris buffered saline (500 mM NaCl) to determine the optimal ratio of labelling and background [. The sec- ondary marker was Protein A-gold (pA G5, BioCell). The gold particles were further enhanced using a silver enhancing Amersham kit. Finally, the thin-sections were transferred on copper-grids, post-stained with 2.5% aque- ous uranyl acetate and examined with a Philips CM 200 Cryo-TEM at an accelerating voltage of 80 kV. To guarantee semi-quantitative comparative labelling, experiments were carried out in parallel on treated and non-treated samples of CBD. Therefore, the exposure to the antibody was identical.
RP carried out the amorphous cellulose, CBD and CBD- FITC production, made the adsorption assays and the image acquisition, participated in the conception of this work and manuscript writing. ALA and ECF helped con- ceiving the image analysis system. MV produced the antiserum. KR was responsible for the TEM-immunolabe- ling experiments. MM is the director of the research unit and helped to draft the manuscript. MG participated in the conception and supervision of the work and contrib- uted to the manuscript preparation. All authors read and approved the final manuscript.
Publish with and every scientist can read your work free of charge
23. Sing K: The use of nitrogen adsorption for the characterisa- tion of porous materials. Colloids and Surfaces A-Physicochemical and Engineering Aspects 2001, 187:3-9.
18. Shoseyov O, Shani Z, Levy I: Microbiol Mol Biol Rev 2006, 70:283-295.
19. Levy I, Shani Z, Shoseyov O: Biomolecular Engineering 2002, 19:17-30.
20. Suurnakki A, Tenkanen M, Siika-aho M, Niku-Paavola ML, Viikari L, Buchert J: Trichoderma reesei cellulases and their core domains in the hydrolysis and modification of chemical pulp.
Cellulose 2000, 7:189-209.
21. Pala H, Lemos MA, Mota M, Gama FM: Enzymatic upgrade of old paperboard containers. Enzyme Microb Technol 2001, 29:274-279.
22. Brunauer S, Emmett PH, Teller E: Adsorption of Gases in Multi- molecular Layers. J Am Chem Soc 1938, 60:309-319.
24. Teeri TT: Crystalline cellulose degradation: New insight into the function of cellobiohydrolases. Trends in Biotechnology 1997, 15:160-167.
16. Maculotti K, Genta I, Perugini P, Imam M, Bernkop-Schnurch A, Pavane Journal of Microencapsulation 2005, 22:459-470.
25. Pinto R, Amaral AL, Carvalho J, Ferreira EC, Mota M, Gama M Biotechnol Prog 2007, 23:1492-1497.
26. Kraulis PJ, Clore GM, Nilges M, Jones TA, Pettersson G, Knowles J, Gronenborn
Biochemistry 1989, 28:7241-7257.
27. Gao PJ, Chen GJ, Wang TH, Zhang YS, Liu J: Acta Biochimica et Biophysica Sinica 2001, 33:13-18.
28. Nigmatullin R, Lovitt R, Wright C, Linder M, Nakari-Setala T, Gama
A: Atomic force microscopy study of cellulose surface inter- action controlled by cellulose binding domains. Colloids and Surfaces B-Biointerfaces 2004, 35:125-135.
29. Ruel K, Ambert K, Joseleau JP: Influence of the enzyme equip- ment of white-rot fungi on the patterns of wood degrada- tion. Fems Microbiology Reviews 1994, 13:241-254.
17. Zeltins A, Schrempf H: Anal Biochem 1995, 231:287-294.
15. Lenkei R, Andersson B: J Immunol Methods 1995, 183:267-277.
"BioMed Central will be the most significant development for disseminating the results of biomedical researc h in our lifetime." Sir Paul Nurse, Cancer Research UK Your research papers will be: available free of charge to the entire biomedical community peer reviewed and published immediately upon acceptance cited in PubMed and archived on PubMed Central yours — you keep the copyright Submit your manuscript here:
6. Mackintosh JA, Veal DA, Karuso P: Proteomics 2005, 5:4673-4677.
Acknowledgements Ricardo Pinto was supported by a grant from the Fundação para a Ciência e a Tecnologia (FCT) SFRH/BD/6934/2001.
1. Nagl S, Schaeferling M, Wolfbeis OS: Fluorescence analysis in microarray technology. Microchimica Acta 2005, 151:1-21.
2. Stewart CN, Millwood RJ, Halfhill MD, Ayalew M, Cardoza V, Kooshki M, Capelle GA, Kyle KR, Piaseki D, McCrum G, Di Benedetto J Journal of Fluorescence 2005, 15:697-705.
3. Sonesson AW, Callisen TH, Brismar H, Elofsson UM: Langmuir 2005, 21:11949-11956.
4. Plant AL, Benson DM, Smith J Cell Biol 1985, 100:1295-1308.
5. Guttman A, Ronai Z, Csapo Z, Gerstner A, Sasvari-Szekely M: Journal of Chromatography A 2000, 894:329-335.
7. Zhang XW, Zhao FL, Li KA: Fluorometric method for the microdetermination of protein using indigo carmine. Micro- chem J 2001, 68:53-59.
14. Bossowski A, Stasiak-Barmuta A, Czarnocka B, Urban M, Dadan J Autoimmunity 2005, 38:605-611.
8. Limon MC, Margolles-Clark E, Benitez T, Penttila M: Fems Microbiology Letters 2001, 198:57-63.
9. Srisodsuk M: Mode of action of Trichoderma reesei cellobiohydrolase I on crystalline cellulose Helsinki, Finland, VTT Publications; 1994:1-107.
10. Pinto R, Carvalho J, Mota M, Gama M: Large-scale production of cellulose-binding domains. Adsorption studies using CBD- FITC conjugates. Cellulose 2006, 13:557-569.
11. Mattinen ML, Linder M, Teleman A, FEBS Lett 1997, 407:291-296.
12. Hilden L, Daniel G, Johansson G:
Biotechnol Lett 2003, 25:553-558.
13. Jervis EJ, Haynes CA, Kilburn DG: J Biol Chem 1997, 272:24016-24023.
30. Ruel K, Faix O, Joseleau JP: New immunogold probes for study- ing the distribution of the different lignin types during plant cell wall biogenesis. Journal of Trace and Microprobe Techniques 1994, 12:247-265.